advertisement

77 P6B 20th International Symposium on Space Terahertz Technology, Charlottesville, 20-22 April 2009 1 Measurement of electron-phonon interaction time of Niobium using heating effect in SIS tunnel junction Boon Kok Tan, Ghassan Yassin, Phichet Kittara and Jamie Leech 160 Abstract—The heating of SIS tunnel junctions by local oscillator (LO) power and bias voltage is well known and has been reported previously. In this paper, we present a novel method for recovering the heating parameters from the experimental pumped I-V curves of an SIS device at 700 GHz, together with the coupled LO power and the embedding impedance. Since this is obtained without assuming a particular power law between LO power and junction temperature, we will be able to find τeph , the electron-phonon interaction time of the superconducting material at various bath temperatures. We would deduce a power law that describes the dependence of the heat flow equation on temperature. 140 120 Current (µA) 100 80 60 40 Index Terms—Superconductor-insulator-superconductor devices, electron-phonon interaction time, heat flow, power law. 20 0 0 Fig. 1. I. I NTRODUCTION N IOBIUM based superconductor-insulator-superconductor (SIS) tunnel junctions are currently the most promising heterodyne mixers for submillimetre radio astronomy below ∼ 1 THz. The performance and characteristic of an SIS mixer near its energy gap is itself an interesting subject to study. Here radiation near the energy gap is strong enough to break the Cooper pairs. A strong dependency of gap voltage on the local oscillator (LO) pumping level can clearly be observed when the mixer is operating in this frequency range. This is commonly related to the heating effects taking place in the device [1], [2]. The implication of the effect on mixer performance is worth studying since accurate determination of the energy gap is central to the performance characteristic of the mixer. In this paper, we present a simple model for studying the heating effects in SIS tunnel junctions near the energy gap, and demonstrate that the electron-phonon interaction time, τeph , of the superconducting material can be directly recovered from the dc pumped I-V curves of an SIS device. II. M ETHOD OF A NALYSIS Our SIS device consists of a Nb-AlOx -Nb junction, sandwiched between the Nb wiring layers and ground plane deposited on quartz substrate across a microstrip line. The junction area is typically 1µm × 1µm with the Nb thickness Boon Kok Tan, Ghassan Yassin and Jamie Leech are with the Department of Physics (Astrophysics), University of Oxford, Denys Wilkinson Building, Keble Road, Oxfordshire, OX1 3RH. (phone: +44 (0)1865 273303; e-mail: tanbk@astro.ox.ac.uk; email: g.yassin1@physics.ox.ac.uk; email: jxl@astro.ox.ac.uk). Phichet Kittara is with Physics Department, Faculty of Science, Mahidol University Bangkok, Bangkok 10400 Thailand. (phone: +66(0)96996479; email: peaw@yahoo.com). Manuscript received 20 April 2009. 0.5 1 1.5 Voltage (mV) 2 2.5 3 The measured I-V curve for different LO pump levels. about 200 nm. The I-V curves measured at different pump levels are shown in Figure 1 and the gap depression with increasing pump level is clearly noted, which is typically in the ∼ 0.1 mV range. The critical temperature of Nb used throughout this paper is assumed to be 9.3 K. The measured curves used in our calculations were obtained using a niobium finline mixer in the frequency range of 650-720 GHz. The Josephson current is suppressed by magnetic field during measurement. Although the heating effect by RF signals for hot electron bolometer (HEB) has been widely studied, there is relatively limited information reported on similar effects in SIS junctions. Leone et. al. [3] has previously reported electron heating of a niobium SIS mixer, using Niobium Titanium Nitrate (NbTiN) stripline with Nb-Al-AlOx -Nb junction. They explained that the mechanism responsible for the heating is the energy gap discontinuity at Nb/NbTiN interface. We, however, believe the heating effect in SIS mixers can result from different mechanisms, although there are some similarities to HEB. As the photon excites quasiparticles to tunnel through the junction barrier, power is dissipated in the junction. In steady state, this power is transfered by thermal conduction through the superconducting ground film to the substrate. For simplicity, we assume that the entire junction is essentially at the same temperature. The heat transfer from the junction to the bath can be described phenomenologically using an effective heat transfer coefficient, α, which may be written as 275 Ptotal = α(Te )wlt(Ten − Tbn ) (1) 20th International Symposium on Space Terahertz Technology, Charlottesville, 20-22 April 2009 77 where Ptotal is the total power coupled the junction, Te is the effective electron temperature (junction temperature), Tb is the bath temperature, wlt is the junction volume and n is an index which depends on the model used for heat transfer. Equation 1 is a rather general equation to describe the heat transfer process. The heat transfer coefficient α(Te ), is a temperature dependent parameter defined as α(Te ) = Ce nTen−1 τeph (3) Recovery of the embedding parameters, including coupled LO power and embedding impedance, are obtained by matching the measured IV-curves with theoretical models based on Werthamer [5] and BCS theory [6]. We have used CalTech’s SuperMix package for this purpose. In recovering the embedding impedance, we have assumed that the heating effect is negligible, which is a reasonable assumption, since we are working with the narrow range of the first photon step. From the BCS equations, the DC and RF power dissipated in the junction at each bias point are given by, n=+∞ X nh̄ω 2 J (eVLO /h̄ω)Idc (V + nh̄ω/e) e n n=−∞ Pdc = Vbias × Idc (4) (5) where Jn is the nth order Bessel function of the first kind and VLO the voltage across the junction associated with the LO power, which is calculated from the recovered LO power from SuperMix. Vbias is the bias voltage and Idc is given by the standard BCS unpumped I-V relation Idc 1 = eRn Z 120 Current (µA) 100 80 40 20 2 2.2 2.4 2.6 2.8 3 Voltage (mV) Fig. 2. The matching of simulated I-V curves with and without the heating effect with the experimental I-V curve. 1. By substituting equation 2 and equation 3 in equation 1, we can then solve for Te . The new gap voltage ∆ is then numerically re-computed using the standard temperature dependent expression, 1 = N (ξF )V Z h̄ωc 0 p tanh( 2kB1 Te ξ 2 + ∆2 ) p dξ ξ 2 + ∆2 (9) where N (ξF ) is the density of states at Fermi level, V is the attractive potential, and h̄ωc is the Debye frequency. It should be noted that the above equation gives a specific value of ∆ at a certain electron temperature, where in reality the I-V curve near the transition is rounded. Since all the junction parameters found using SuperMix are normalized to the gap voltage, the theoretical current calculated using the previously recovered LO power and embedding impedance, is simply the product of the normalized 2 /Rn . current from SuperMix and the gap current given as Vgap This entire process is repeated throughout the whole range of bias voltages. The generated I-V curve is then compared to the measured curve, and the parameters are optimized until both theoretical and measured curves are matched. III. R ESULT AND D ISCUSSION ∞ N (ξ)N (ξ − eV )[f (ξ − eV ) − f (ξ)]dξ (6) −∞ where Rn is the junction normal state resistance, f (ξ) is the Fermi-Dirac distribution function and N (ξ) describes the density of states. Note that both functions, f (ξ) and N (ξ), are explicit functions of the voltage-dependence electron temperature, in our case, ξ N (ξ) = p 2 ξ − ∆2 (Te ) f (ξ) = Experiment Curve Theoretical Curve without Heating Theoretical Curve with Heating 60 −∆ 2N (ξF )∆2 exp Te kB T e Prf = 140 (2) where Ce is the electron heat capacity and τeph is the electron-phonon interaction time. In order to incorporate the temperature dependence effect of the heat capacity into the final equation, the low temperature limit heat capacity equation is used to calculate Ce [4]. Ce = 2 1 exp kBξTe + 1 . (7) (8) We start with an initial guess of τeph and index n, and use equation 5 and equation 4 to give Ptotal into equation Figure 2 shows the I-V response of our SIS junction using the highest pumping level curve shown in figure 1. Also in the figure we show the theoretical I-V curves calculated using embedding parameters recovered by the SuperMix model with and without the heating effect. The curve with heating is simulated using the value of τeph = 7.8 ns and index n = 4. The glitch in the heated curve near the knee of the gap voltage is probably due to the electron temperature being calculated without the rounding of the gap voltage in BCS equation, as noted previously. This can potentially be corrected by incorporating the imaginary lifetime-broadening parameter in the density of states equation [7], [8]. Unfortunately, the value of this parameter for Nb is difficult to obtain from the literature. This sudden step change is also seen in figure 3, where Te , gap voltage and power across the junction are plotted as a function of bias voltage. 276 20th International Symposium on Space Terahertz Technology, Charlottesville, 20-22 April 2009 77 600 results also show that the heat transfer equation does not depend significantly on the index n. 5.5 5 400 4.5 300 4 200 3.5 100 3 0 R EFERENCES Gap Voltage (mV), Temperature (K) Heating Power (nW) Total Power Gap Voltage Electron Temperature 500 2.5 0 0.5 1 1.5 2 Bias Voltage (mV) 2.5 3 3.5 Fig. 3. The heating power coupled to the junction as a function of bias voltage. Shown together are the junction temperature and the gap voltage change corresponding to the bias voltage. 10 τeph(ns) 9 8 [1] B. Leone, B. D. Jackson, J. R. Gao, and T. M. Klapwijk, “Geometric heat trapping in niobium superconductor-insulator-superconductor mixers due to niobium titanium nitride leads,” Applied Physics Letters, vol. 76, no. 6, pp. 780–782, 2000. [2] P. Dieleman, T. M. Klapwijk, S. Kovtonyuk, and H. van de Stadt, “Direct current heating in superconductorinsulatorsuperconductor tunnel devices for thz mixing applications,” Applied Physics Letters, vol. 69, no. 3, p. 418, 1996. [3] B. Leone, J. R. Gao, T. M. Klapwijk, B. D. Jackson, and W. M. L. amd G. de Lange, “Hot electron effect in terahertz hybrid devices,” IEEE Transactions on Applied Superconductivity, vol. 11, no. 1, pp. 649–652, 2001. [4] T. V. Duzer and C. W. Turner, Principles of superconductive devices and circuits. New York, Oxford: Elsevier, 1981. [5] N. R. Werthamer, “Nonlinear self-coupling of josephson radiation in superconducting tunnel junctions,” Physical Review, vol. 147, pp. 255– 263, 1966. [6] J. Bardeen, L. Cooper, and J. Schrieffer, “Theory of superconductivity,” Physical Review, vol. 108, no. 5, pp. 1175–1204, 1957. [7] R. C. Dynes, V. Narayanamurti, and J. P. Garno, “Direct measurement of quasiparticle-lifetime broadening in a strong-coupled superconductor,” Phys. Rev. Lett., vol. 41, no. 21, pp. 1509–1512, 1978. [8] B. Mitrovi and L. A. Rozema, “On the correct formula for the lifetime broadened superconducting density of states,” Journal Physics: Condense Matter, vol. 20, pp. 15 215–15 218, 2008. 7 6 4 3.5 3 2.5 2 1.5 1 3 5 Index n Fig. 4. Contour of the error surface with different guess value of τeph and index n. Figure 4 shows the error surface contour of different guess value of n and τeph . It is clear from the figure that the change in n had little effect on the error surface. In other words, the index n is not as significant as τeph . This can easily be explained if we assume the difference between Te and Tb is small compared to Te and Tb . The term (Ten − Tbn )/nTen−1 can then be approximated as Te − Tb without index n in the final equation. It should be noted that heating parameters can also be recovered solely from the unpumped I-V curve. A procedure similar to the one described above can be employed, with the junction model replaced by a modified temperature dependence polynomial equation. The results obtained in this method can be compared with those obtained using the pumped I-V curve to give better constrains on the heating parameters recovered. IV. C ONCLUSION We present a simple model for measuring parameter of a superconductor by recovering the change in the electron temperature from the experimentally pumped I-V curve. Our 277